- Nano Express
- Open Access
Cycling-Induced Capacity Increase of Graphene Aerogel/ZnO Nanomembrane Composite Anode Fabricated by Atomic Layer Deposition
Nanoscale Research Letters volume 14, Article number: 69 (2019)
Zinc oxide (ZnO) nanomembranes/graphene aerogel (GAZ) composites were successfully fabricated via atomic layer deposition (ALD). The composition of GAZ composites can be controlled by changing the number of ALD cycles. Experimental results demonstrated that the anode made from GAZ composite with ZnO nanomembrane of 100 ALD cycles exhibited highest specific capacity and best rate performance. A capacity increase of more than 2 times during the first 500 cycles was observed, and a highest capacity of 1200 mAh g−1 at current density of 1000 mA g−1 was observed after 500 cycles. On the basis of detailed electrochemical investigations, we ascribe the remarkable cycling-induced capacity increase to the alloying process accompanied by the formation of a polymer layer resulting from kinetically activated electrolyte degradation at low voltage regions.
Lithium-ion batteries (LIBs) have been the dominant power source for consumer electronics due to their safety, high energy density, and low self-discharge [1,2,3,4]. However, graphite carbon as the traditional anode material delivers a charge-discharge capacity of 372 mAh g−1, which is not the promising anode material for the upcoming electric vehicles. It is urgent to develop new anode materials with high specific capacity to satisfy the ever-increasing demand in electric vehicles. Non-graphitic carbons such as graphene [5, 6], transition metal oxides (ZnO [7, 8], Fe2O3 [9, 10], Co3O4 [11, 12], MnO2 ), and their composites [14,15,16] have been the promising substitutes for graphite as anode materials.
ZnO has attracted much attention which is attributed to its high theoretic capacity (978 mAh/g, nearly two times higher than that of graphite), high lithium-ion diffusion efficiency, low cost, and environmental friendliness [17, 18]. However, ZnO suffers from large volume expansion/contraction (~ 163%) and poor conductivity, thus leading to fast capacity fading and poor cycling performance [8, 19]. Various strategies have been promoted to solve these problems, including the use of ZnO nanostructures (nanorod arrays  and nanosheets ) and carbon-based composites [21, 22]. Zhao et al.  fabricated three-dimensional carbon/ZnO nanomembrane composite foam through an immersing process. The composites could maintain more than 92% of the initial capacity after 700 cycles at 2 A g−1 because of the flexibility of ZnO nanomembranes and the effective electron/ion transport through carbon foam. In our previous work, we also successfully synthesized ZnO/expanded graphite composite and it could deliver a capacity of 438 mAh g−1 at 200 mA g−1 after 500 cycles . In addition, graphene is considered as an excellent anode material with outstanding chemical stability, flexibility, and conductivity . Graphene aerogel (GA), the 3D architectures of assembled 2D graphene sheets, not only keeps the advantage of the unique structure of graphene sheets, but also possesses ultralow density, high and tunable porosity, excellent mechanical strength, and extraordinary adsorption properties [25, 26]. We consider that the unique 3D structure of GA combined with ZnO nanomembranes may have advantageous applications in anodes for LIBs.
Herein, we designed an electrode structure with 3D GA coated with ZnO nanomembranes (GAZ). GA was firstly fabricated via a template-free, freeze-drying strategy and then coated with ZnO nanomembranes via atomic layer deposition (ALD) . The components of GAZ composites can be easily tuned by changing the number of ALD cycles, which has been demonstrated in our previous researches [27,28,29,30]. In the composite, GA works as conductive skeletons and supports for ZnO nanomembranes. Its flexible nature helps to accommodate the volume change of ZnO during discharge/charge process, and the porous structure facilitates effective Li+ transport. Thus, when applied for lithium storage, the GAZ composites demonstrate high specific capacity and excellent rate performance; the composites deliver a reversible capacity of 1200 mAh g−1 at 1000 mA g−1 after 500 cycles. A notable capacity increase phenomenon was also observed in the charge-discharge process of the composites. Testing results confirm that the cycling-induced capacity increase can be attributed to the formation of a polymer layer in low voltage regions. We believe that the mechanism can be utilized to explain the similar phenomenon in other metal oxides.
Synthesis of GA
Graphene oxide (GO) used in this work was prepared from natural graphite using a modified Hummers’ method . All chemicals were obtained from Sinopharm Chemical Reagent Co. Ltd., China. In a typical procedure for preparing the graphene hydrogel, 5.0 mg dopamine was added into the GO water dispersion followed by vigorous stirring for 10 min to obtain uniform solution. Fifteen milligrams l-ascorbic acid was added into the mixture with vigorous magnetic stirring until it was completely dissolved. Thirdly, the mixture was sealed in a glass vessel and heated at 95 °C for 10 h to transform the brown aqueous solution into a black graphene hydrogel. Next, the hydrogel was placed on a metal plate, which in turn rested in a pool of liquid nitrogen after dialysis in water to remove soluble species. The hydrogel was totally frozen by directional freezing from the metal-hydrogel interface to the top surface. And then, the aerogel was obtained from the frozen hydrogel by freeze-drying. The dry aerogel was placed in a glass vessel filled with perfluorooctyltriethoxysilane (PFOES)/ethanol (2 wt.%) with no direct contact between the liquid and the aerogel. Finally, the sealed glass vessel was heated at 70 °C for 8 h. GA could be obtained after thorough drying in air.
Preparation of GAZ Composite
The obtained GA was coated with ZnO nanomembranes in the ALD chamber with dimethylzinc and deionized water as zinc and oxidant sources, respectively. The chamber temperature during deposition period was 150 °C. A typical ALD cycle includes diethylzinc pulse (30 ms), waiting time (3 s), and nitrogen (N2) purge (15 s) and water pulse (30 ms), waiting time (3 s), and N2 purge (15 s). N2 served as both the carrier gas and purge gas at a flow rate of 30 sccm. The precursors used were purchased from J&K Scientific Ltd., China. The thicknesses of ZnO nanomembranes in the composites were tuned by changing the number of ALD cycles: 20, 100, and 300 cycles (shorted as GAZ20, GAZ100 and GAZ300). Then, the samples were annealed in tube furnace at 700 °C for 120 min in N2 atmosphere. For comparison, pure GA was also annealed in tube furnace at 700 °C for 120 min in N2 atmosphere.
The morphologies and microstructures of the GAZ composites were examined using scanning electron microscopy (SEM, Zeiss Sigma) and transmission electron microscope (TEM, Nova NanoSem 450). The X-ray diffractometer (XRD) patterns were recorded using a Bruker D8A Advance XRD with Cu Kα radiation (λ = 1.5405 Å). The composition of GAZ composites was tested by energy dispersive spectroscopy (EDS) attached to SEM.
The electrochemical tests were accessed on a CR2016 coin cell with lithium metal acting as both the counter and reference electrode. The working electrode was composed of 80 wt.% active material (i.e., GAZ composites), 10 wt.% conductive additive agent (Super P), and 10 wt.% binder (polyvinylidene difluoride in N-methyl-2-pyrrolidone (NMP)). The electrolyte used was a solution of 1 M LiPF6 dissolved in ethylene carbonate/diethyl carbonate (EC/DEC, 1:1 v/v). The cells were assembled in an argon-filled glove box (H2O, O2 < 1 ppm). Galvanostatic measurements were performed on a battery testing system (LAND CT2001A) in the voltage range of 0.01–3 V. The current rates used were based on the total mass of the electrode. Cyclic voltammetry (CV) tests were also carried out at a scan rate of 0.1 mV s−1 from 0.001 to 3 V using a Zennium/IM6 electrochemical workstation.
Results and Discussion
The fabrication schematic of GAZ composites is depicted in Fig. 1a. GA was synthesized by a template-free, freeze-drying strategy. Then, ALD was utilized to decorate GA surface with ZnO nanomembranes. The morphology and microstructure of GA and GAZ were demonstrated by means of SEM. Figure 1b clearly shows that GA was made up of graphene nanosheets. Figure 1c–e displays the microstructural similarities and differences in GAZ composites with the increasing number of ALD cycles. One can see that ZnO nanomembranes are well deposited on the GA surfaces, yet the surface coverages are quite different. The graphene layers in GAZ20 are not completely coated by ZnO nanomembranes (Fig. 1c). The ZnO was distributed as dots/islands on GA surface due to the lack of reactive sites or functional groups on GA surface . When the number of ALD cycles is increased to 100, the surface of GA is entirely decorated with ZnO nanomembrane consisting of small nanoparticles, as shown in Fig. 1d. Figure 1e and the corresponding enlarged image in the inset demonstrates that a thick and dense ZnO nanomembrane was formed with more ALD cylces. SEM images in Fig. 1 demonstrate that the ZnO coverage on GA surface increases correspondingly with the increasing ALD cycles.
EDS analyses were used to determine the chemical compositions of GAZ composites. As shown in the inset of Fig. 2a, the existence and atom percentages of O and Zn indicate that ZnO nanomembranes were successfully decorated on the GA surface which is consistent with the SEM images. The atomic percentage of Zn in GAZ as s function of ALD cycles is illustrated in Fig. 2a, and an obvious increase of Zn concentration is observed, which indicates the composition of the composites can be easily tuned by changing ALD cycles. To investigate the crystal structure of these composites, the composites were characterized by XRD and the results are shown in Fig. 2b. For GAZ300 and GAZ100, the characteristic diffraction peaks of ZnO (100), (002), (101), (102), (110), (103), (112), and (201) are clearly exhibited in XRD patterns (PDF#36–1451) , suggesting that ZnO nanomembranes coated on GA surfaces can maintain the hexagonal wurtzite structure. However, very weak diffraction peaks can be distinguished in GAZ20 because the content of ZnO is too low. With the increasing number of ALD cycles, the characteristic peak of ZnO is more obvious due to higher ZnO concentration. The experimental results in Fig. 2 further prove that the composition of the composite is successfully tuned by changing the ALD cycles; thus, the influence of the composition on device performance can be easily probed.
The rate performance of pure GA and GAZ composites with different ALD cycles was evaluated at various current densities (1000–2500 mA g−1 as depicted in Fig. 3a). Both current density and capacity were calculated based on total mass of the electrode. GA20 shows stable capacity at even high current density (2.5 A g−1). As the number of ALD cycles increases to 100, the GAZ100 electrode shows better rate performance. As the current density increases to 1500, 2000, and 2500 mA g−1, the GAZ100 electrode exhibits the capacity of 520, 450, and 400 mAh g−1, respectively. When the current density returns back to 1000 mAh g−1, the GAZ100 electrode recovers the initial reversible capacity of 600 mAh g−1. The excellent rate performance is attributed to the good conductivity, porous structure, and mechanical flexibility of GA, which facilitate the fast e−/Li+ transport in the composite electrode and alleviate ZnO pulverization. One may note that the initial discharge capacity of pure GA is higher than its theoretical capacity. The extra capacity was attributed to the decomposition of electrolyte to form the solid electrolyte interphase (SEI) layer . When the number of ALD cycles increases to 300, the GAZ300 delivers lower capacity and shows worse rate performance than GAZ100. Therefore, rate performance is not positively correlated with the number of ALD cycles. We infer that the low content of ZnO in GAZ20 leads to the lower charge-discharge capacity. As ALD cycles increases to 300, the resistance of the composite increases correspondingly, and the thicker ZnO nanomembranes entirely covered the GA surface, which is not beneficial for electrolyte penetration and lithium-ion transmission. In addition, the volume change of thicker ZnO cannot be well relaxed in GAZ300. As a result, the rate performance of GAZ300 deteriorates although it possesses a higher ZnO content.
To investigate the specific capacity in more detail, we took a long-cycle test of pure GA and GAZ composites at current rate of 1000 mA g−1 for 1000 cycles after the rate performance test, and the results are illustrated in Fig. 3b. The specific capacity of GAZ composites obviously increased from 50th to 500th cycles. It is noted that capacity increases from 580 mAh g−1 to 1200 mAh g−1 for GAZ100, from 450 to 700 mAh g−1 for GAZ300, from 300 to 600 mAh g−1 for GAZ20. Correspondingly, the highest areal capacity of GAZ100 is 0.61 mA/cm2, which is higher than those of GAZ20 (0.31 mAh/cm2) and GAZ300 (0.35 mAh/cm2). However, the capacity of pure GA in the long cycle only shows a small capacity increase, and ZnO also did not show obvious capacity increase in previous research [7, 23, 32]. This indicates that the capacity increase in GAZ composites should result from the co-effect of ZnO and GA components. Such a capacity increase phenomenon in cycling process has been observed in anodes made from many metal oxides [9, 33,34,35,36,37] and was ascribed to the formation of reversible polymer layer due to activated electrolyte degradation . Previous literatures [16, 38, 39] have proved that the layer can effectively store the Li-ions and the capacity is therefore enhanced.
To further investigate the capacity increase phenomenon, we carried out CV test of GAZ100 electrode. Figure 4a illustrates the CV profiles of the GAZ100 electrode of the 1st, 300th, and 800th cycles, which were recorded with the potential window of 0.01–3.0 V at the scanning rate 0.1 mV s−1. In the first cycle, four cathodic peaks located at 1.6 V (I), 0.9 V (II), 0.2 V (III), and 0.06 V (IV) were observed. The peak positioned at 1.6 V (I) could be associated with the formation of the SEI layer [19, 40]. The peaks observed at 0.9 (II) and 0.2 V (III) correspond to the reduction of ZnO to Zn (ZnO + Li+ + 6e− → Zn + Li2O) and the alloying process (xLi + Zn → LixZn), respectively [19, 32, 41,42,43]. In addition, the strong reduction peak closed to 0.06 V (IV) is related to the lithiation process of GA [15, 44]. Compared with the first cycle, the cathodic peaks at 1.6 V (I) after 300 cycles still exists indicating that the formation of SEI layer still occurred in subsequent long cycles. However, the peak at 1.6 V (I) disappears after 800 cycles, indicating the stable formation of SEI layers. The reduction peaks at 0.9 (II) and 0.2 V (III) shift to 0.62 and 0.3 V, respectively, after 300 and 800 charge/discharge cycles. On the basis of the aforementioned discussion, we attributed this shift to the reduction reactions of ZnO to Zn accompanied by the formation of the polymer layer [9, 45, 46], as will be discussed later. As for the anodic curve, five peaks at 0.2, 0.5, 1.3, 1.7, and 2.3 V are observed. The oxidation peaks at 0.2, 0.5, and 1.3 V correspond to the multi-step dealloying process of the LixZn alloy to form Zn, and the peaks at 1.7 and 2.3 V correspond to the oxidation of Zn to generate ZnO [7, 47]. In subsequent cycles, it can be clearly seen that all these anodic peaks shift to higher voltages. It indicates the faster electron transport or slower deintercalation of lithium ion in GAZ100 anode in subsequent cycles. However, the expansion/contraction of ZnO in charge/discharge cycles should cause relatively worse contact with GA, resulting in slower electron transport. Thus, the observed peak shift to higher voltage should be mainly ascribed to the slower deintercalation of lithium ion. Previous literature has demonstrated that the formation of the polymer layer would increase the interfacial resistance and the deintercalation of lithium ion would be hindered . In addition, it is worth noting that the integrated area of anodic and cathodic peaks increases with the cycles (Fig. 4a), which is consistent with the increased capacity shown in Fig. 3b.
Figure 4b demonstrates the selected discharge voltage profiles of the 1st and the 500th cycles of GAZ100. The corresponding capacity increment is shown in the inset of Fig. 4b. It is demonstrated that most capacity increment was gained at 0.02–0.9 V. According to the CV illustrated in Fig. 4a, the discharge process can be divided into four stages based on the four voltage ranges of 3.0–1.6, 1.6–0.9, 0.9–0.2, and 0.2–0.06 V, corresponding to the formation of SEI layer, reduction of ZnO to Zn, alloying process accompanied by the formation of the polymer layer, and lithiation process of GA, respectively. As described in Fig. 4b, ∆C1, ∆C2, ∆C3, and ∆C4 are the capacity increments of the respective voltage ranges from the 1st to 500th cycle. The total capacity increase (from the 1st to the 500th cycles, 589.1 mAh g−1, ∆C4) consists of the growing capacity from the SEI layer formation (44.4 mAh g−1, ∆C1), ZnO reduction to Zn (80.4 mAh g−1, ∆C2 − ∆C1), the alloying process of Zn and Li (258 mAh g−1, ∆C3 − ∆C2), and the GA lithiation process (206.3 mAh g−1, ∆C4 − ∆C3). Obviously, the major capacity increase (∆C3 − ∆C2) mainly occurred in the low potential ranges, where the polymer layer may form, as described in previous literatures [49, 50]. In addition, we consider that the gradual exposure of active material (i.e., GAZ composites) to electrolyte after charge/discharge cycles may also partially contribute to the capacity increase (∆C4 − ∆C3).
The morphology of GAZ100 electrode after 500 cycles was investigated in detail to prove the stability of the electrodes. Typical TEM image of GAZ100 electrode after 500 charge/discharge cycles is shown in Additional file 1: Figure S1, and the crystal lattice of ZnO can be clearly observed. The TEM results shown in Additional file 1: Figure S1 indicate that the ZnO nanocrystals did not crack after 500 cycles, suggesting a stable performance of current composite .
In summary, GAZ composites were easily synthesized via ALD. The composition of GAZ could be finely tuned by changing the number of ALD cycles. Characterization demonstrates that the electrodes made from composites exhibit better rate performance and higher capacity because the composite combines the excellent conductivity and flexibility of GA with high specific capacity of ZnO nanomembranes. A remarkable capacity increase with cycling (from 580 mAh/g to 1200 mAh/g for GAZ100 electrode) was observed in GAZ composites. Detailed electrochemical analyses suggest that the phenomenon is caused by the formation of polymer layer at low voltage region, which can storage more lithium so that the reversible capacity was higher. The convenient fabrication process and high reversible capacity of the GAZ composites make them promising anode materials for future LIBs.
Atomic layer deposition
Energy dispersive spectroscopy
Zinc oxide/graphene aerogel
Solid electrolyte interphase
Scanning electron microscopy
Transmission electron microscope
Tarascon JM, Armand M (2001) Issues and challenges facing rechargeable lithium batteries. Nature 414(6861):359–367
Etacheri V, Marom R, Elazari R, Salitra G, Aurbach D (2011) Challenges in the development of advanced Li-ion batteries: a review. Energy Environ Sci 4(9):3243–3262
Xu W, Wang JL, Ding F, Chen XL, Nasybutin E, Zhang YH, Zhang JG (2014) Lithium metal anodes for rechargeable batteries. Energy Environ Sci 7(2):513–537
Goriparti S, Miele E, De Angelis F, Di Fabrizio E, Zaccaria RP, Capiglia C (2014) Review on recent progress of nanostructured anode materials for Li-ion batteries. J Power Sources 257:421–443
Yoo E, Kim J, Hosono E, Zhou H, Kudo T, Honma I (2008) Large reversible Li storage of graphene nanosheet families for use in rechargeable lithium ion batteries. Nano Lett 8(8):2277–2282
Singh V, Joung D, Zhai L, Das S, Khondaker SI, Seal S (2011) Graphene based materials: past, present and future. Prog Mater Sci 56(8):1178–1271
Huang XH, Xia XH, Yuan YF, Zhou F (2011) Porous ZnO nanosheets grown on copper substrates as anodes for lithium ion batteries. Electrochim Acta 56(14):4960–4965
Lu S, Wang H, Zhou J, Wu X, Qin W (2017) Atomic layer deposition of ZnO on carbon black as nanostructured anode materials for high-performance lithium-ion batteries. Nanoscale 9(3):1184–1192
Li X, Qiao L, Li D, Wang X, Xie W, He D (2013) Three-dimensional network structured a-Fe2O3 made from a stainless steel plate as a high-performance electrode for lithium ion batteries. J Mater Chem A 1:6400–6406
Wang P, Ding H, Bark T, Chen C (2007) Nanosized α-Fe2O3 and Li–Fe composite oxide electrodes for lithium-ion batteries. Electrochim Acta 52(24):6650–6655
Li Y, Tan B, Wu Y (2008) Mesoporous CO3O4 nanowire arrays for lithium ion batteries with high capacity and rate capability. Nano Lett 8(1):265–270
Lou X, Deng D, Lee J, Feng J, Archer LA (2008) Self-supported formatnion of needlelike Co3O4 nanotubes and their application as lithium-ion battery electrodes. Adv Mater 20(2):258
Shi Y, Guo B, Corr SA, Shi Q, Hu Y, Heier KR, Chen L, Seshadri R, Stucky GD (2009) Ordered mesoporous metallic MoO2 materials with highly reversible lithium storage capacity. Nano Lett 9(12):4215–4220
Xiao L, Wu D, Han S, Huang Y, Li S, He M, Zhang F, Feng X (2013) Self-assembled Fe2O3/graphene aerogel with high lithium storage performance. ACS Appl Mater Inter 5(9):3764–3769
Wang R, Xu C, Sun J, Gao L (2015) Three-dimensional Fe2O3 nanocubes/nitrogen-doped graphene aerogels: nucleation mechanism and lithium storage properties. Sci Rep 4:7171
Cho S, Jung J, Kim C, Kim I (2017) Rational design of 1-D Co3O4 nanofibers@low content graphene composite anode for high performance Li-ion batteries. Sci Rep 7:45015
Zhang J, Gu P, Xu J, Xue H, Pang H (2016) High performance of electrochemical lithium storage batteries: ZnO-based nanomaterials for lithium-ion and lithium-sulfur batteries. Nanoscale 8(44):18578–18595
Quartarone E, Dall'Asta V, Resmini A, Tealdi C, Tredici IG, Tamburini UA, Mustarelli P (2016) Graphite-coated ZnO nanosheets as high-capacity, highly stable, and binder-free anodes for lithium-ion batteries. J Power Sources 320:314–321
Yu M, Wang A, Wang Y, Li C, Shi G (2014) An alumina stabilized ZnO-graphene anode for lithium ion batteries via atomic layer deposition. Nanoscale 6(19):11419–11424
Zhang G, Hou S, Zhang H, Zeng W, Yan F, Li CC, Duan H (2015) High-performance and ultra-stable lithium-ion batteries based on MOF-derived ZnO@ZnO quantum dots/C core-shell nanorod arrays on a carbon cloth anode. Adv Mater 27(14):2400–2405
Zhao YT, Huang GS, Li YL, Edy R, Gao PB, Tang H, Bao ZH, Mei YF (2018) Three-dimensional carbon/ZnO nanomembrane foam as an anode for lithium-ion battery with long-life and high areal capacity. J Mater Chem A 6(16):7227–7235
Zhao YT, Huang GS, Wang DR, Ma Y, Fan ZY, Bao ZH, Mei YF (2018) Sandwiched porous C/ZnO/porous C nanosheet battery anodes with stable solid-electrolyte interphase for fast and long cycling. J Mater Chem A 6:22870–22878
Li YL, Zhao YT, Huang GS, Xu BR, Wang B, Pan RB, Men CL, Mei YF (2017) ZnO nanomembrane/expanded graphite composite synthesized by atomic layer deposition as binder-free anode for lithium ion batteries. ACS Appl Mater Inter 9(44):38522–38529
Bonaccorso F, Colombo L, Yu G, Stoller M, Tozzini V, Ferrari AC, Ruoff RS, Pellegrini V (2015) Graphene, related two-dimensional crystals, and hybrid systems for energy conversion and storage. Science 347(6217):1246501–1246509
Sun H, Xu Z, Gao C (2013) Multifunctional, ultra-flyweight, synergistically assembled carbon aerogels. Adv Mater 25(18):2554–2560
Garakani MA, Abouali S, Zhang B, Takagi CA, Xu Z, Huang J, Huang J, Kim J (2014) Cobalt carbonate/and cobalt oxide/graphene aerogel composite anodes for high performance Li-ion batteries. ACS Appl Mater Inter 6(21):18971–18980
Edy R, Huang GS, Zhao YT, Guo Y, Zhang J, Mei YF, Shi JJ (2017) Influence of reactive surface groups on the deposition of oxides thin film by atomic layer deposition. Surf Coat Technol 329:149–154
Edy R, Huang GS, Zhao YT, Zhang J, Mei YF, Shi JJ (2016) Atomic layer deposition of TiO2-nanomembrane-based photocatalysts with enhanced performance. AIP Adv 6(11):115113
Edy R, Zhao YT, Huang GS, Shi JJ, Zhang J, Solovev AA, Mei YF (2016) TiO2 nanosheets synthesized by atomic layer deposition for photocatalysis. Prog Nat Sci Mater Int 26(5):493–497
Pan SQ, Zhao YT, Huang GS, Wang J, Baunack S, Gemming T, Schmidt OG, Mei YF (2015) Highly photocatalytic TiO2 interconnected porous powder fabricated by sponge-templated atomic layer deposition. Nanotechnology 26(36):364001
Kim D, Kang H, Kim JM, Kim H (2011) The properties of plasma-enhanced atomic layer deposition (ALD) ZnO thin films and comparison with thermal ALD. Appl Surf Sci 257(8):3776–3779
Xie Q, Zhang X, Wu X, Wu H, Liu X, Yue G, Yang Y, Peng D (2014) Yolk-shell ZnO-C microspheres with enhanced electrochemical performance as anode material for lithium ion batteries. Electrochim Acta 125:659–665
Chou S, Wang J, Wexler D, Konstantinov K, Zhong C, Liu H, Dou S (2010) High-surface-area a-Fe2O3/carbon nanocomposite: one-step synthesis and its highly reversible and enhanced high-rate lithium storage properties. J Mater Chem 20:2092–2098
Wu Z, Ren W, Wen L, Gao L, Zhao J, Chen Z, Zhou G, Li F, Cheng H (2010) Graphene anchored with Co3O4 nanoparticles as anode of lithium ion batteries with enhanced reversible capacity and cyclic performance. ACS Nano 4(6):3187–3194
Wang L, Yu Y, Chen PC, Zhang DW, Chen CH (2008) Electrospinning synthesis of C/Fe3O4 composite nanofibers and their application for high performance lithium-ion batteries. J Power Sources 183(2):717–723
Zhou J, Song H, Ma L, Chen X (2011) Magnetite/graphene nanosheet composites: interfacial interaction and its impact on the durable high-rate performance in lithium-ion batteries. RSC Adv 1(5):782–791
Adelhelm P, Hu Y, Antonietti M, Maier J, Smarsly BM (2009) Hollow Fe-containing carbon fibers with tubular tertiary structure: preparation and Li-storage properties. J Mater Chem 19(11):1616
Lee KT, Cho J (2011) Roles of nanosize in lithium reactive nanomaterials for lithium ion batteries. Nano Today 6(1):28–41
Laruelle S, Grugeon S, Poizot P, Dolle M, Dupont L, Tarascon JM (2002) On the origin of the extra electrochemical capacity displayed by MO/Li cells at low potential. J Electrochem Soc 149(5):627–634
Tu Z, Yang G, Song H, Wang C (2016) Amorphous ZnO quantum dot/mesoporous carbon bubble composites for a high-performance lithium-ion battery anode. ACS Appl Mater Inter 9(1):439–446
Wang R, Xu C, Sun J, Liu Y, Gao L, Lin C (2013) Free-standing and binder-free lithium-ion electrodes based on robust layered assembly of graphene and Co3O4 nanosheets. Nanoscale 5(15):6960
Zou F, Hu X, Li Z, Qie L, Hu C, Zeng R, Jiang Y, Huang Y (2014) MOF-derived porous ZnO/ZnFe2O4/C octahedra with hollow interiors for high-rate lithium-ion batteries. Adv Mater 26(38):6622–6628
Rui X, Tan H, Sim D, Liu W, Xu C, Hng HH, Yazami R, Lim TM, Yan Q (2013) Template-free synthesis of urchin-like Co3O4 hollow spheres with good lithium storage properties. J Power Sources 222:97–102
Tan C, Cao J, Khattak AM, Cai F, Jiang B, Yang G, Hu S (2014) High-performance tin oxide-nitrogen doped graphene aerogel hybrids as anode materials for lithium-ion batteries. J Power Sources 270:28–33
Meng J, Cao Y, Suo Y, Liu Y, Zhang J, Zheng X (2015) Facile fabrication of 3D SiO2@graphene aerogel composites as anode material for lithium ion batteries. Electrochim Acta 176:1001–1009
Wang X, Li X, Sun X, Li F, Liu Q, Wang Q, He D (2011) Nanostructured NiO electrode for high rate Li-ion batteries. J Mater Chem 21(11):3571
Liu H, Shi L, Li D, Yu J, Zhang H, Ullah S, Yang B, Li C, Zhu C, Xu J (2018) Rational design of hierarchical ZnO@carbon nanoflower for high performance lithium ion battery anodes. J Power Sources 387:64–71
Do J, Weng C (2005) Preparation and characterization of CoO used as anodic material of lithium battery. J Power Sources 146(1–2):482–486
Wang X, Yang Z, Sun X, Li X, Wang D, Wang P, He D (2011) NiO nanocone array electrode with high capacity and rate capability for Li-ion batteries. J Mater Chem 21(27):9988
Ponrouch A, Palacín MR (2012) Optimisation of performance through electrode formulation in conversion materials for lithium ion batteries: Co3O4 as a case example. J Power Sources 212:233–246
The authors acknowledge the contributions of Fei Ma and Zhe Zhao in the device testing.
This work is supported by the Natural Science Foundation of China (Nos. 61628401 and U1632115), Science and Technology Commission of Shanghai Municipality (No. 17JC1401700), and the Changjiang Young Scholars Program of China. Part of the work is also supported by the National Key Technologies R&D Program of China (No. 2015ZX02102-003).
The authors declare that they have no competing interests.
Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional affiliations.
About this article
Cite this article
Wang, D., Li, Y., Zhao, Y. et al. Cycling-Induced Capacity Increase of Graphene Aerogel/ZnO Nanomembrane Composite Anode Fabricated by Atomic Layer Deposition. Nanoscale Res Lett 14, 69 (2019) doi:10.1186/s11671-019-2900-7
- Zinc oxide
- Graphene aerogel
- Atomic layer deposition
- Capacity increase
- Lithium-ion batteries